Presentation on theme: "1 Nam Tran Lead Research Engineer. 2 Overview Methods of incorporating GTR Applications of rubber-modified binders Performance of test sections at NCAT."— Presentation transcript:
4 Two methods for incorporating GTR into HMA Wet process GTR acts as a binder modifier (up to 20% of total binder) 2 processes: asphalt-rubber and terminal blend Dry process GTR acts as a rubber aggregate (1-3% of aggregate)
5 Asphalt-Rubber > 15% crumb rubber passing #8 or #10 mesh Reacted sufficiently to cause swelling of rubber 2 types of asphalt-rubber binders Type I (used in AZ and TX) 18-20% crumb rubber Type II (used in CA) about 20% rubber 75% tire rubber and 25% natural rubber May include up to 6% heavy aromatic oils Both types blended at elevated temp (>350 o F) in low shear system for at least 45 minutes
6 Terminal Blend 5-20% crumb rubber passing #40 or #80 mesh Blended in refinery or stationary asphalt terminal with little or no agitation Can contain polymers All components heated over extended period of time to dissolve rubber particles Used in Arizona, California, Florida, Texas, and several northeastern states
7 Asphalt Rubber vs. Terminal Blend Asphalt Rubber Rubberized Asphalt Terminal Blend 1,500-2,500 centipoises at 375°F, extremely viscous 1,500-2,500 centipoises at 375°F, extremely viscous 300-600 centipoises at 325°F, significantly less viscous than AR 300-600 centipoises at 325°F, significantly less viscous than AR Rubber Pavements Association
8 Asphalt Rubber vs. Terminal Blend Use more crumb rubber Requires special equipment to produce Longer documented history of performance Mostly uses recipe specs Not cost effective in small quantities Cannot be PG graded Use less crumb rubber Does not require special equipment Shorter documented history Many are proprietary Rubber usage more difficult to document Can be PG graded
11 Caltrans Reduced Thickness Design Guideline Developed in 1992 based on laboratory and long-term field data (two decades) Uses a deflection based design method Up to 50 % reduction in thickness compared to conventional AC design thickness Over 1000 reduced thickness projects
12 Major Rubber-Modified Asphalt Users California ARSC (AR chip seal) SAMI-R RHMA-O RHMA-G RHMA-D Florida ARMI (SAMI) GTR modified-OGFC (FC-5) GTR modified-DGFC Texas AR Chip Seals AR Underseal (SAMI) CRM-PFC CRM-HMAC Arizona SAM SAMI ARFC ARAC
South Carolina Florida North Carolina Washington, D.C. Delaware New Jersey Connecticut Rhode Island Massachusetts Maine New Hampshire Vermont New York Ohio Kentucky West Virginia Pennsylvania Indiana Illinois Iowa Missouri Arkansas Tennessee Georgia Alabama Mississippi Louisiana Texas Oklahoma Nebraska Kansas South Dakota North Dakota Virginia New Mexico Arizona Colorado Utah Nevada California Alaska Minnesota Wisconsin Michigan Montana Wyoming Idaho Oregon Washington Maryland Hawaii Rubber used Not using rubber States where Asphalt-Rubber has been used (DOT, Transportation Authority, County or City) Puerto Rico Rubber Pavements Association
21 IDT (10, 0, -20 o C) S6 Strength @ 10 o C: 4,394,770 psi Critical cracking temperature: -24.4 o C True PG of binder: 76.6-26.3 S7 Strength @ 10 o C: 4,667,902 psi Critical cracking temperature: -25 o C True PG of binder: 81.7-25
22 On-going Testing Rutting and moisture damage resistance Flow number Hamburg Cracking resistance Energy Ratio
26 National and Regional Levels PG grading of rubber modified asphalt FHWA binder ETG is working on a test method Determining rubber content No proposed method Use of GTR-modified asphalt with WMA Asphalt rubber Terminal blend
27 National and Regional Levels Recyclability of GTR-modified asphalt mixtures Incorporating GTR-modified mixtures in mechanistic pavement designs E* predictive models Mechanistic and transfer models Can we save up to 50% in thickness compared to conventional AC design thickness?
28 Regional and State Levels What are your questions or concerns when specifying GTR-modified binder mixtures and/or accepting new GTR-blending technologies?